Reinforcement of TiB2 Nanoparticles in Aluminium Piston Alloys for High Performance at Elevated Temperature
- 79 Downloads
Nano-TiB2 particles produced by in situ approaches were employed to reinforce the Mahle 174 piston alloy. Experimental results showed that, with TiB2 nanoparticles, the mechanical properties were significantly improved at ambient and elevated temperatures. The ultimate tensile property at room temperature was increased from 250 to 332 MPa. The ultimate tensile property at 300 °C was increased from 121 to 174 MPa, and that at 350 °C was increased from 86 to 116 MPa. The increase was 82 MPa at ambient temperature, 53 MPa at 300 °C and 30 MPa at 350 °C, respectively. The mechanism of property improvement in the nanocomposites is attributed to the well-distributed nanoparticles in Al matrix, thermal stability of TiB2 at high temperature and the formation of high density of dislocation network in the vicinity of TiB2/Al interface.
KeywordsNanocomposites Piston alloy Microstructure Mechanical property High-temperature properties
Piston components produced by Al alloys have been extensively achieved in industry to obtain light weighting in transport manufacturing. The increasingly restricted demands of low emission of internal combustion engines require a high explosion pressure and working temperature in the cylinder chambers, which results in the increase in service temperature and mechanical properties of piston up to 400 °C. Therefore, piston alloys with high strength above 300 °C are attracting more and more attention. In general, the strengthening at elevated temperature mainly results from grain boundary strengthening, precipitation strengthening and secondary phase strengthening. The elements such as Si, Fe, Cu and Ni form intermetallic and eutectic phases along grain boundaries to contribute the grain boundary strengthening and secondary phase strengthening. The elements such as Mg, Cu, V and Zr can form very fine precipitates in the Al matrix for precipitation strengthening . In the currently used pistons, Al–Si alloys are popular due to their good castability and acceptable durability and machinability, in which the Mg and Cu are the best and economic elements employed to enhance the anti-deformation capability of Al piston alloys. The Mg2Si and Al2Cu are two key phases formed as secondary phases in grain boundaries and as precipitates within α-Al matrix for strengthening. The Mg2Si can improve the high-temperature property up to 180 °C, and Al2Cu can improve the high-temperature property up to 300 °C. Above the critical temperature, these phases will become unstable and grow quickly with prolonged time at high temperature and subsequently lose their strengthening advantages in the piston alloys.
To further improve the mechanical properties of Al piston alloys at high temperature, it is necessary to reinforce the alloy by fine precipitates that are stable and no obviously growth at high temperature. Particle-reinforced metal matrix composites (MMCs) are the capable materials and good candidates to provide good mechanical properties above 300 °C because of the existence of ceramic particles in the matrix, such as SiC, AlN and TiB2. It was reported that the creep resistance of the Al composites increases with increasing volume fraction of SiC reinforcement [2, 3]. The experimental results of Ma et al. revealed that the Al composite containing AlN particles has excellent ultimate tensile strength at both the room temperature and the high temperature of 350 °C . The Al composites reinforced by TiB2 particles possessed the good ultimate tensile strength at high temperature between 300 and 400 °C [5, 6]. However, in the as-cast microstructure, most of the ceramic particles formed by in situ or ex situ approaches are located in the grain boundary after solidification, showing the significant non-uniform distribution and therefore not beneficial for the mechanical properties. Consequently, the challenge is how to obtain the well-distributed particles in the Al matrix, of which the refinement of primary aluminium phase is an effective way. Nano-TiB2 particles have been proved to be able to act as nucleation sites during solidification to effectively refine the grain size of primary Al phase [7, 8, 9]. In reality, the addition of 0.2 wt% Al5Ti1B master alloy into aluminium alloys as grain refiner is a common practice in casting manufacturing , by which only 0.0064 wt% TiB2 particles are introduced into Al melt. The amount of TiB2 particle is significantly insufficient as the reinforcement phase for the strengthening at high temperature.
Therefore, in the present study, we tried to investigate the influence of nano-TiB2 particles on the mechanical properties of the Mahle 174 piston alloy at different temperatures. About 5 wt% nano-TiB2 particles were produced by in situ technology in the Mahle 174 piston alloy as reinforcement phases for high temperature. The mechanisms of the property improvement in the nanocomposites are discussed in association with the relationship between the nanoprocessing, microstructure and mechanical properties.
Mahle 174 alloy (11%Si, 3.5%Cu, 2%Ni, 0.6%Mg, 0.15%Zr, 0.15%V and 0.15%Ti) was employed as matrix alloy to produce nano-TiB2-reinforced composite. In situ technology of chemical reactions between K2TiF6, KBF4 and Al at 850 °C for 1 h was used to prepare TiB2 particles. In the liquid state of K2TiF6, KBF4 and Al at 850 °C, three reactions occurred to synthesize TiB2 particle. [Ti] was extracted from the reaction between K2TiF6 and Al, and [B] was extracted from the reaction between KBF4 and Al. Then, [Ti] and [B] were combined together to form TiB2 particles. After the completion of the reaction process, the rotary degassing was used to purify the melt and then the melt was poured into the tensile sample mould designed according to ASTM-557 standard.
All samples were subjected to the T6 heat treatment, in which the samples were solutionized at 515 °C for 2 h and immediately quenched into the water at ambient temperature; after 24-h stabilization at room temperature, the samples were aged at 170 °C for 10 h. The tensile properties were tested using an Instron 5500 testing machine at different temperatures. The ramp rate was 1 mm/min. For high-temperature testing, the samples were held for 30 min to homogenize the sample temperature at the given temperature before testing. Samples for microstructure analysis were prepared following the standard procedure. Scanning electron microscopy (SEM) and transmission electron microscopy (TEM) were employed to observe the microstructure.
3 Results and Discussion
Grain refinement has been recognized as an effective strengthening approach in Al alloys [11, 12]. In the experimental alloys, the grain size of the as-cast microstructure had the same level in these two alloys. Therefore, the grain refinement strengthening did not contribute to the improvement of mechanical properties. Precipitation strengthening is mainly influenced by the morphology and the size of the precipitates formed during heat treatment which is determined by the alloy composition and heat treatment process. In the present study, the same condition in the alloy composition, casting process and heat treatment of Mahle 174 and TiB2/Mahle 174 indicated that there was no obvious difference of the contribution of the precipitation strengthening on the improvement of the UTS. For the Al composites reinforced by nanoparticles, the high density of dislocation network could be formed in the vicinity of the interface between the reinforcement and the matrix. These dislocations could be generated by the high thermal stress during solidification and heat treatment process because of the difference of the coefficient of thermal expansion between the nanoparticles and the base alloy.
For particles-reinforced Al composites, the interface between the reinforcement phase and the matrix plays an important role in the enhancement of mechanical properties. The good bonding will benefit the property improvement, whilst the bad bonding should minimize or avoid through the control of synthesis process. The common defects on the interface between particle and matrix are non-bonding and/or the existence of the brittle secondary phases.
The property improvement of piston alloys at high temperature can be achieved by employing nano-TiB2 particles as reinforcements to produce Mahle 174 composite. The ultimate tensile strength at room temperature was increased from 250 to 332 MPa. The ultimate tensile strength at 300 °C was increased from 121 to 174 MPa, and that at 350 °C was increased from 86 to 116 MPa. The improvement was attributed to the well-distributed particles in Al matrix and the dislocation strengthening caused by nanoparticles.